Section 0472-00-04 Architectural Cast Stone
This specification encompasses basic requirements for Cast Stone, a refined architectural
concrete building unit manufactured to simulate natural cut stone, used in unit masonry
applications. Cast Stone is a masonry product, used as an architectural feature, trim,
ornament or facing for buildings or other structures.
Part 1 General
1.1 FABRICATOR: The Fabricator shall have a minimum of 5 years successful
experience in fabrication of integrally colored architectural Cast Stone units, similar to
units required for this project.
A. Continental Stone Company; 159 Harvest Road, Reidsville, NC, 27320. Tel:
(336) 951-2945. Fax: (336) 951-3555.
Email: firstname.lastname@example.org Web:
B. Any fabricator that can submit certifications, literature and test reports showing
that they can meet the requirements of this specification.
Section Includes - Architectural Cast Stone.
1.2. Related Sections
Section – 01 33 00 – Submittal Procedures.
Section – 04 05 13 – Masonry Mortaring...
Section – 04 05 16 – Masonry Grouting.
Section – 04 05 19 – Masonry Anchorage and Reinforcing.
Section – 07 90 00 – Joint Protection.
ACI 318 – Building Code Requirements for Reinforced Concrete.
ASTM A 185 - Standard Specification for Steel Welded Wire Reinforcement,
Plain, for Concrete.
ASTM A 615/A 615M - Standard Specification for Deformed and Plain Billet-
Steel Bars for Reinforced Concrete.
ASTM C 33 – Standard Specification for Concrete Aggregates.
ASTM C 150 - Standard Specification for Portland Cement.
ASTM C 173 - Standard Test Method for Air Content of Freshly Mixed Concrete
by the Volume Method.
ASTM C 231 - Standard Test Method for Air Content of Freshly Mixed Concrete
by the Pressure Method.
ASTM C 260 - Standard Specification for Air-Entrained Admixtures for
ASTM C 270 - Standard Specification for Mortar for Unit Masonry.
ASTM C 426 – Standard Test Method for Linear Shrinkage of Concrete Masonry
ASTM C 494/C 494M - Standard Specification for Chemical Admixtures for
ASTM C 618 – Specification for Coal Fly Ash and Raw or Calcined Natural
Pozzolan for Use as a Mineral Admixture in Concrete.
ASTM C 666 – Standard Test Method for Resistance of Concrete to Rapid
Freezing and Thawing.
ASTM C 979 - Standard Specification for Coloring Pigments for Integrally
ASTM C 989 – Standard Specification for Ground Granulated Blast-Furnace Slag
for Use in Concrete.
ASTM C 1194 - Standard Test Method for Compressive Strength of Architectural
ASTM C 1195 - Standard Test Method for Absorption of Architectural Cast
ASTM C 1364 - Standard Specification for Architectural Cast Stone.
ASTM D 2244 – Standard Test Method for Calculation of Color Differences from
Instrumentally Measured Color Coordinates.
Cast Stone Institute® Technical Manual (Current Edition)
Cast Stone - a refined architectural concrete building unit manufactured to
simulate natural cut stone, used in unit masonry applications.
o Dry Cast Concrete Products - manufactured from zero slump concrete.
Vibrant Dry Tamp (VDT) casting method: Vibratory ramming of
earth moist, zero- slump concrete against a rigid mold until it is
Machine casting method: manufactured from earth moist, zero-
slump concrete compacted by machinery using vibration and
pressure against a mold until it becomes densely consolidated.
o Wet Cast Concrete Products - manufactured from measurable slump
Wet casting method: manufactured from measurable slump
concrete and vibrated into a mold until it becomes densely
1.5. Submittal Procedures
Comply with Section 01 33 00 – Submittal Procedures.
Samples: Submit pieces of the Cast Stone that are representative of the general
range of finish and color proposed to be furnished for the project.
Test results: Submit manufacturers test results of Cast Stone previously made by
Shop Drawings: Submit manufacturers shop drawings including profiles, cross-
sections, reinforcement, exposed faces, arrangement of joints (optional for
standard or semi-custom installations), anchoring methods, anchors (if required),
annotation of stone types and their location.
1.6. Quality Assurance
o Manufacturer shall have sufficient plant facilities to produce the shapes,
quantities and size of Cast Stone required in accordance with the project
o Manufacturer shall submit a written list of projects similar in scope and at
least three (3) years of age, along with owner, architect and contractor
Standards: Comply with the requirements of the Cast Stone Institute® Technical
Manual and the project specifications. Where a conflict may occur, the contract
documents shall prevail.
Mock-up (Optional) Provide full size unit(s) for use in construction of sample
wall. The approved mock-up shall become the standard for appearance and
workmanship for the project.
Part 2 Products
2.1. Architectural Cast Stone
Comply with ASTM C 1364
Physical properties: Provide the following:
o Compressive Strength - ASTM C 1194: 6,500 psi (45 Mpa) minimum for
products at 28 days.
o Absorption - ASTM C 1195: 6% maximum by the cold water method, or
10% maximum by the boiling method for products at 28 days.
o Air Content – ASTM C173 or C 231, for wet cast product shall be 4-8%
for units exposed to freeze-thaw environments. Air entrainment is not
required for VDT products.
o Freeze-thaw – ASTM C 1364: The CPWL shall be less than 5% after 300
cycles of freezing and thawing.
o Linear Shrinkage – ASTM C 426: Shrinkage shall not exceed 0.065%.
Job site testing – One (1) sample from production units may be selected at random
from the field for each 500 cubic feet (14 m 3) delivered to the job site.
o Three (3) field cut cube specimens from each of these samples shall have
an average minimum compressive strength of not less than 85% with no
single specimen testing less than 75% of design strength as allowed by
o Three (3) field cut cube specimens from each of these samples shall have
an average maximum cold-water absorption of 6%.
o Field specimens shall be tested in accordance with ASTM C 1194 and C
2.2. Raw Materials
Portland cement – Type I or Type III, white and/or grey, ASTM C 150.
Coarse aggregates - Granite, quartz or limestone, ASTM C 33, except for
gradation, and are optional for the VDT casting method.
Fine aggregates - Manufactured or natural sands, ASTM C 33, except for
Colors - Inorganic iron oxide pigments, ASTM C 979 except that carbon black
pigments shall not be used.
Admixtures- Comply with the following:
o ASTM C 260 for air-entraining admixtures.
o ASTM C 494/C 495M Types A - G for water reducing, retarding,
accelerating and high range admixtures.
o Other admixtures: integral water repellents and other chemicals, for which
no ASTM Standard exists, shall be previously established as suitable for
use in concrete by proven field performance or through laboratory testing.
o ASTM C 618 mineral admixtures of dark and variable colors shall not be
used in surfaces intended to be exposed to view.
o ASTM C 989 granulated blast furnace slag may be used to improve
physical properties. Tests are required to verify these features.
Water – Potable
o ASTM A 615/A 615M. Grade 40 or 60 steel galvanized or epoxy coated
when cover is less than 1.5 in. (37 mm).
o Welded Wire Fabric: ASTM A 185 where applicable for wet cast units.
All anchors, dowels and other anchoring devices and shims shall be standard
building stone anchors commercially available in a non-corrosive material such as
zinc plated, galvanized steel, brass, or stainless steel Type 302 or 304.
2.3. Color And Finish
Match sample on file in architect’s office.
All surfaces intended to be exposed to view shall have a fine-grained texture
similar to natural stone, with no air voids in excess of 1/32 in. (0.8 mm) and the
density of such voids shall be less than 3 occurrences per any 1 in.2 (25 mm2) and
not obvious under direct daylight illumination at a 5 ft (1.5m) distance.
Units shall exhibit a texture approximately equal to the approved sample when
viewed under direct daylight illumination at a 10 ft (3 m) distance.
o ASTM D 2244 permissible variation in color between units of comparable
age subjected to similar weathering exposure.
Total color difference – not greater than 6 units.
Total hue difference – not greater than 2 units.
Minor chipping resulting from shipment and delivery shall not be grounds for
rejection. Minor chips shall not be obvious under direct daylight illumination
from a 20-ft (6 m) distance.
The occurrence of crazing or efflorescence shall not constitute a cause for
Remove cement film, if required, from exposed surfaces prior to packaging for
Reinforce the units as required by the drawings and for safe handling and
Minimum reinforcing shall be 0.25 percent of the cross section area.
Reinforcement shall be noncorrosive where faces exposed to weather are covered
with less than 1.5 in. (38 mm) of concrete material. All reinforcement shall have
minimum coverage of twice the diameter of the bars.
Panels, soffits and similar stones greater than 24 in. (600 mm) in one direction
shall be reinforced in that direction. Units less than 24 in. (600 mm) in both their
length and width dimension shall be non-reinforced unless otherwise specified.
Welded wire fabric reinforcing shall not be used in dry cast products.
A. Cure units in a warm curing chamber approximately 100ºF (37.8ºC) at 95
percent relative humidity for approximately 12 hours, or cure in a 95 percent
moist environment at a minimum 70ºF (21.1ºC) for 16 hours after casting.
Additional yard curing at 95 percent relative humidity shall be 350 degree-days
(i.e. 7 days @ 50°F (10°C) or 5 days @ 70°F (21°C)) prior to shipping. Form
cured units shall be protected from moisture evaporation with curing blankets or
curing compounds after casting.
2.6. Manufacturing Tolerances
Cross section dimensions shall not deviate by more than ±1/8 in. (3 mm) from
Length of units shall not deviate by more than length/ 360 or ±1/8 in. (3 mm),
whichever is greater, not to exceed ±1/4 in. (6 mm).
o Maximum length of any unit shall not exceed 15 times the average
thickness of such unit unless otherwise agreed by the manufacturer.
Warp, bow or twist of units shall not exceed length/ 360 or ±1/8 in. (3 mm),
whichever is greater.
Location of dowel holes, anchor slots, flashing grooves, false joints and similar
features – On formed sides of unit, 1/8 in. (3 mm), on unformed sides of unit, 3/8
in. (9 mm) maximum deviation.
2.7. Production Quality Control
o Test compressive strength and absorption from specimens selected at
random from plant production.
o Samples shall be taken and tested from every 500 (14 m3) cubic feet of
o Perform tests in accordance ASTM C 1194 and C 1195.
o New and existing mix designs shall be tested for strength and absorption
compliance prior to producing units.
2.8. Delivery, Storage And Handling
Mark production units with the identification marks as shown on the shop
Package units and protect them from staining or damage during shipping and
Provide an itemized list of product to support the bill of lading.
3. Delivery, Storage And Handling
Installing contractor shall check Cast Stone materials for fit and finish prior to
installation. Do not set unacceptable units.
3.2. Setting Tolerances
Comply with Cast Stone Institute® Technical Manual.
Set stones 1/8 in. (3 mm) or less, within the plane of adjacent units.
Joints, plus - 1/16 in. (1.5 mm), minus - 1/8 in. (3 mm).
o At stone/brick joints 3/8 in. (9.5 cm).
o At stone/stone joints in vertical position 1/4 in. (6 mm) (3/8 in. (9.5 mm)
o Stone/stone joints exposed on top 3/8 in. (9.5 mm).
o Mortar, Type N, ASTM C 270.
o Use a full bed of mortar at all bed joints.
o Flush vertical joints full with mortar.
o Leave all joints with exposed tops or under relieving angles open for
o Leave head joints in copings and projecting components open for sealant.
Location of joints:
o As shown on shop drawings.
o At control and expansion joints unless otherwise shown.
Drench units with clean water prior to setting.
Fill dowel holes and anchor slots completely with mortar or non-shrink grout.
Set units in full bed of mortar, unless otherwise detailed.
Rake mortar joints 3/4 in. (18 mm) in. for pointing.
Remove excess mortar from unit faces immediately after setting.
Tuck point unit joints to a slight concave profile.
3.5. Joint Protection
Comply with requirements of Section 07 90 00.
Prime ends of units, insert properly sized backing rod and install required sealant.
3.6. Repair and Cleaning
Repair chips with touchup materials furnished by manufacturer.
Saturate units to be cleaned prior to applying an approved masonry cleaner.
Consult with manufacturer for appropriate cleaners
3.7. Inspection and Acceptance
Inspect finished installation according to Bulletin #36.
Do not field apply water repellant until repair, cleaning, inspection and
acceptance is completed.